Electrical

Property | Temperature | Value |
---|---|---|

Electrical resistivity | 20.0 °C | 2.63E-7 Ω·m Show Material materials with Electrical resistivity of 2.63E-7 Ω·m |

100.0 °C | 3.08E-7 Ω·m Show Material materials with Electrical resistivity of 3.08E-7 Ω·m | |

200.0 °C | 3.78E-7 Ω·m Show Material materials with Electrical resistivity of 3.78E-7 Ω·m | |

300.0 °C | 4.66E-7 Ω·m Show Material materials with Electrical resistivity of 4.66E-7 Ω·m | |

400.0 °C | 5.69E-7 Ω·m Show Material materials with Electrical resistivity of 5.69E-7 Ω·m | |

500.0 °C | 6.87E-7 Ω·m Show Material materials with Electrical resistivity of 6.87E-7 Ω·m | |

600.0 °C | 8.26E-7 Ω·m Show Material materials with Electrical resistivity of 8.26E-7 Ω·m | |

General

Property | Temperature | Value |
---|---|---|

Density | 20.0 °C | 7.81 - 7.85 g/cm³ Show Material materials with Density of 7.81 - 7.85 g/cm³ |

Mechanical

Property | Temperature | Value |
---|---|---|

Elastic modulus | -100.0 °C | 217 GPa Show Material materials with Elastic modulus of 217 GPa |

0.0 °C | 213 GPa Show Material materials with Elastic modulus of 213 GPa | |

20.0 °C | 212 GPa Show Material materials with Elastic modulus of 212 GPa | |

100.0 °C | 207 GPa Show Material materials with Elastic modulus of 207 GPa | |

200.0 °C | 199 GPa Show Material materials with Elastic modulus of 199 GPa | |

300.0 °C | 192 GPa Show Material materials with Elastic modulus of 192 GPa | |

400.0 °C | 184 GPa Show Material materials with Elastic modulus of 184 GPa | |

500.0 °C | 175 GPa Show Material materials with Elastic modulus of 175 GPa | |

600.0 °C | 164 GPa Show Material materials with Elastic modulus of 164 GPa | |

Unlock all property charts | ||

Hardness, Brinell | 20.0 °C | 207 [-] Show Material materials with Hardness, Brinell of 207 [-] |

Poisson's ratio | 20.0 °C | 0.28 [-] Show Material materials with Poisson's ratio of 0.28 [-] |

Thermal

Property | Temperature | Value |
---|---|---|

Coefficient of thermal expansion | -100.0 °C | 1.05E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.05E-5 1/K |

0.0 °C | 1.14E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.14E-5 1/K | |

20.0 °C | 1.15E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.15E-5 1/K | |

100.0 °C | 1.21E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.21E-5 1/K | |

200.0 °C | 1.27E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.27E-5 1/K | |

300.0 °C | 1.32E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.32E-5 1/K | |

400.0 °C | 1.36E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.36E-5 1/K | |

500.0 °C | 1.4E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.4E-5 1/K | |

600.0 °C | 1.44E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.44E-5 1/K | |

Unlock all property charts | ||

Specific heat capacity | -100.0 °C | 423 J/(kg·K) Show Material materials with Specific heat capacity of 423 J/(kg·K) |

0.0 °C | 456 J/(kg·K) Show Material materials with Specific heat capacity of 456 J/(kg·K) | |

20.0 °C | 461 J/(kg·K) Show Material materials with Specific heat capacity of 461 J/(kg·K) | |

100.0 °C | 479 J/(kg·K) Show Material materials with Specific heat capacity of 479 J/(kg·K) | |

200.0 °C | 499 J/(kg·K) Show Material materials with Specific heat capacity of 499 J/(kg·K) | |

300.0 °C | 517 J/(kg·K) Show Material materials with Specific heat capacity of 517 J/(kg·K) | |

400.0 °C | 536 J/(kg·K) Show Material materials with Specific heat capacity of 536 J/(kg·K) | |

500.0 °C | 558 J/(kg·K) Show Material materials with Specific heat capacity of 558 J/(kg·K) | |

600.0 °C | 587 J/(kg·K) Show Material materials with Specific heat capacity of 587 J/(kg·K) | |

Unlock all property charts | ||

Thermal conductivity | 20.0 °C | 39.6 W/(m·K) Show Material materials with Thermal conductivity of 39.6 W/(m·K) |

100.0 °C | 41.6 W/(m·K) Show Material materials with Thermal conductivity of 41.6 W/(m·K) | |

200.0 °C | 41.8 W/(m·K) Show Material materials with Thermal conductivity of 41.8 W/(m·K) | |

300.0 °C | 40.3 W/(m·K) Show Material materials with Thermal conductivity of 40.3 W/(m·K) | |

400.0 °C | 38.2 W/(m·K) Show Material materials with Thermal conductivity of 38.2 W/(m·K) | |

500.0 °C | 36 W/(m·K) Show Material materials with Thermal conductivity of 36 W/(m·K) | |

600.0 °C | 33.6 W/(m·K) Show Material materials with Thermal conductivity of 33.6 W/(m·K) | |

Unlock all property charts | ||

Thermal diffusivity | 20.0 °C | 11000 mm²/s Show Material materials with Thermal diffusivity of 11000 mm²/s |

100.0 °C | 10800 mm²/s Show Material materials with Thermal diffusivity of 10800 mm²/s | |

200.0 °C | 10100 mm²/s Show Material materials with Thermal diffusivity of 10100 mm²/s | |

300.0 °C | 9200 mm²/s Show Material materials with Thermal diffusivity of 9200 mm²/s | |

400.0 °C | 8100 mm²/s Show Material materials with Thermal diffusivity of 8100 mm²/s | |

500.0 °C | 7000 mm²/s Show Material materials with Thermal diffusivity of 7000 mm²/s | |

600.0 °C | 5700 mm²/s Show Material materials with Thermal diffusivity of 5700 mm²/s | |

Unlock all property charts |

Chemical properties

Property | Value |
---|---|

Carbon | 0.14 - 0.19 % Show Material materials with Carbon of 0.14 - 0.19 % |

Chromium | 0.8 - 1.1 % Show Material materials with Chromium of 0.8 - 1.1 % |

Copper | 0.3 % Show Material materials with Copper of 0.3 % |

Manganese | 1 - 1.3 % Show Material materials with Manganese of 1 - 1.3 % |

Phosphorus | 0.04 % Show Material materials with Phosphorus of 0.04 % |

Silicon | 0.4 % Show Material materials with Silicon of 0.4 % |

Sulfur | 0.035 % Show Material materials with Sulfur of 0.035 % |